• date post

11-Apr-2018
• Category

## Documents

• view

221

5

Embed Size (px)

### Transcript of Phase Transformation - - Phase transformation Phase transformation â€“ Formation of...

• Phase Transformation

• Phase transformationPhase transformation Formation of a new phase having a distinct physical/chemical character and/or a different structure than the parent phase.It involves two phenomena Nucleation and Growth Nucleation formation of a nucleus or tiny particles of the new phase.A nucleus is formed when the Gibbs free energy, G, of the system decreases i.e. G becomes negative.Two types of nucleation Heterogeneous and HomogeneousGrowth Increase in size of the nucleus at the expense of the parent phase.

• Homogeneous nucleationIn homogeneous nucleation the probability of nucleation is same throughout the volume of the parent phase. The simplest example of nucleation is solidification of a metal.Above melting point Tm, liquid free energy, Gl < Gs (Solid free energy) and free energy change for solidification G > 0. Below Tm, G < 0 and nuclei of the solid phase form.

• Homogeneous nucleationThere are two contributions to free energy change, volume free energy Gv and surface free energy, due to creation of a new surface.Taking the nucleus as a spherical particle of radius r

G = 4/3r3Gv + 4r2 ------------------ (1)The tiny particle of the solid that forms first will be stable only when it achieves a critical radius (r*). Below the critical radius it is unstable and is called embryo.Since this happens at the maximum of the G vs. r curve dG /dr = 4r2Gv + 8r = 0This yields and

vGr

2* 23

)(316*

vGG

• Heterogeneous nucleationHere, the probability of nucleation is much higher at certain preferred sites such as mold wall, inclusions, grain boundaries, compared to rest of the parent phase. Example - Solidification of a liquid on an inclusion surface

vSLG

r

2

*

)(*)coscos32()(3

4* 323

SGG

G HomvHet

The small value of ensures that the energy barrier (G) is effectively lowered in heterogeneous nucleation.

With a similar approach it can be shown that and

IL = IS + SL cos

• Nucleation and Growth KineticsOnce the embryo exceeds the critical size r*, the growth of the nucleus starts. Nucleation continues simultaneously.Nucleation and growth rates are function of temp. Nucleation rate increases with cooling rate and degree of undercooling (T = Tm T). High nucleation rate and low growth Finer grain size.The over all transformation rate is the product of nucleation and growth rates.

• Fe-C Phase diagram

• Phases in Fe-C system-ferrite Interstitial solid solution of C in BCC iron. Max solubility of C is 0.025%. Exists from 273C to 910C. Austenite () - Interstitial solid solution of C in FCC iron. Max solubility of C is 2.1%. Exists from 910C - 1394C. -ferrite (BCC) exists over the temp range of 1394C to 1539C. Max solubility of C is 0.09%.Cementite, Fe3C - is an intermetallic compound. C content in Fe3C is 6.67%.Graphite, the free form of C, also exists in the Fe-C system.Bainite (B) is another phase which forms in steels at higher cooling rates.The hard phase martensite (M) forms below the bainitic temperature range at high cooling rates.

• Critical temperatures in Fe-C systemThe eutectoid temperature (727C) during heating and cooling is Ac1 and Ar1 respectively. A for arrt (arrest), c for chauffage (heating) and r for refroidissement (cooling). At normal rates of heating or cooling Ac1 > Ar1.A2 at 768 C is the currie temp above which Fe turns paramagnetic while heating.The temperatures corresponding to ( +)/ and ( +Fe3C)/phase boundaries are function of carbon content and are represented as A3 and Acm respectively. The eutectic temperature is 1146 C.The peritectic temperature is at 1495 C.

• Phase transformation in Fe-C systemPeritectic reaction at 1495 C L (0.53% C) + (0.09% C) (0.17% C)Eutectic reaction at 1146CL (4.3% C) (2.1 % C) + Fe3C (6.67% C). The eutectic mixture of austenite () and cementite (Fe3C) is called Ledeburite. Compositions right and left of 4.3% are called hyper and hypoeutectic steels (Cast iron) respectively. Eutectoid reaction at 727C (0.8 % C) (0.025% C) + Fe3C (6.67% C). The eutectoid mixture of ferrite () and cementite (Fe3C) is called Pearlite. Compositions right and left of 0.8% are called hyper and hypoeutectoid steels respectively. Compositions up to 2.1% C are steels and beyond this it is considered as cast iron.

• MicrostructuresA eutectoid steel (0.8% C) will have 100% pearlite (p) at room temperature (RT). The pearlite formed under equilibrium conditions consists of alternate lamellas of ferrite and Fe3C.

Schematic of Pearlite White areas are

Hypoeutectoid steels + p; hypereutectoid Fe3C + p. Hypoeutectic cast irons consist of + ledeburite (Le) below the eutectic temp and p + Fe3C + Le at RT as the transforms to Fe3C and p at the eutectoid temp. Similarly hyper eutectic cast irons will have a structure of Fe3C + Le.

• T-T-T diagramThe relation between temperature and time for the formation of a phase is given by T-T-T or temp time transformation diagrams also known as isothermal-transformation diagram. A typical T-T-T diagram is shown below. The phases formed on isothermal holding at a given temp for a certain period of time are indicated.

• T-T-T diagramAt normal cooling rates pearlite (P) forms, higher cooling rates generates bainite (B). The size of pearlite or bainite depends on the transformation temp. Martensite (M) forms when the steel is cooled below the maternsite start (Ms) temp at much higher cooling rate so that the nose of the T-T-T curve (shown dotted) is avoided (the long blue arrow) .Diffusion rates below Ms is so low that M transformation is a diffusionless process (the C content remains same). However, the crystal structure changes from FCC () to body centered tetragonal (BCT).

• C-C-T diagramIn actual practice a steel is generally cooled continuously. Continuous-cooling-transformation (C-C-T) diagrams depict this situation. The C-C-T curve (Blue) is shifted to the right of the T-T-T (dashed) curve as continuous cooling transformation occurs at lower temperature and longer time compared isothermal holding.

• C-C-T diagramBainite generally does not form in steels during continuous cooling and hence the C-C-T curve ceases just below the nose.The microstructure (fine or coarse) depends on the cooling rate. Higher the cooling rate finer the microstructure is.Finer size pearlite is called sorbite and very fine size pearlite is called troostite.The critical cooling rate is the one at which the cooling curve just touches the nose of the C-C-T curve.A cooling rate higher than the critical rate is needed to form martensite.

• ExamplesEx.1. A eutectoid steel is slowly cooled from 750 C to a temperature just below 727 C . Calculate the percentage of ferrite and cementite.Solution: Eutectoid composition 0.8% C, Ferrite composition - 0.025% C and cementite 6.67% C.Apply the lever rule to get the percentages as% Ferrite = 100* (6.67 0.80)/(6.67 0.025) = 88.3%%Cementite = 100* (0.80 0.025)/(6.67 0.025) = 11.7%

Ex.2. A carbon steel cooled from austenitic region contains 9.1% ferrite. What is the C content in the steel?

Let c be C content. Apply the lever rule0.091 = (6.67 c)/(6.67 0.025) c = 0.1% C

• References

Key words. Phase transformation; Nucleation; Homogeneous and heterogeneous nucleation; Growth; Fe-C phase diagram; Eutectoid reaction; T-T-T diagram; C-C-T diagram

• Quiz1. What are the different stages of phase transformation?2. What are homogeneous and heterogeneous nucleation?3. Derive the expression for critical radius of the nucleus?4. What are the different phases present in the Fe-C system?5. How many invariants reactions are present in the Fe-C

system and what are those?6. What are microstructure of eutectoid, hypoeutectoid and

hypereuctectoid steels obtained under equilibrium conditions?

7. What are T-T-T and C-C-T diagrams? What is the fundamental difference between them?

8. What should be the conditions for forming martensite in steels?

9. Why is the martensitic transformation in steels a diffusionless process?

• Quiz10. What are sorbite and troostite?11. A plain-carbon steel contains 93 wt% ferrite and 7 % Fe3C.

What is the average carbon content in the steel?12. A 0.9% C steel is slowly cooled from 900 C to a

temperature just below 727 C . Calculate the percentages of proeutectoid cementite and eutectoid ferrite?

13. A 0.4% C steel is slowly cooled from 940 C to (A) just above 727 C (B) just below 727 C.Calculate the amount of austenite and proeutectoid ferrite for case (A).Calculate the amount of proeutectoid ferrite and eutectoid ferrite and cementite for case (B).